dye sensitized solar cell ( dssc ) is a new derivative of a solar cell , developed by grtzel . it is based on semiconductor electrode - adsorbed dye , a counter electrode , and an electrolyte containing iodide and triiodide ions . this device is capable of generating energy by converting the light absorbed into electrical energy . previously , it has been reported that the highest efficiency from a metal as sensitizer has been achieved from a compound containing ruthenium , with a total of 11 - 12% efficiency . recent findings have found that perovskite sensitized solar cells have achieved a power conversion efficiency of approximately 15% . although such results provide better efficiency and high durability , the advantages are often offset by their high cost of production , complicated synthetic routes , environmental impact , and the tendency to undergo degradation in presence of water . in contrast , the natural organic dyes are widely available and involve simple preparation , nontoxic , and complete biodegradation . the use of nontoxic natural pigments as sensitizer would definitely enhance the environmental and economic benefits of this alternative form of solar energy conversion . due to these reasons , natural dyes are becoming attractive inexpensive candidates for renewable energy resources . the natural dye sensitizer may still produce very low efficiency , but with continuous advanced studies and research , improvisation of the efficiency of dsscs has become a reality and hopeful . anthocyanins are the most abundant , naturally occurring flavonoid pigments which often give a bright red , blue , or violet color to plant petals , fruits , and stems . sometimes , they are present in a range of tissues including roots , tubers , and stems . since anthocyanin shows the red to blue color of the visible spectrum , it is considered as one of the best sensitizers for wide bandgap semiconductors . although anthocyanin pigments are abundant in plants , isolated anthocyanin pigments are highly instable and degradable . their stability is affected by several factors including ph , storage temperature , and sunlight exposure levels . hence , it is important to evaluate the optimum conditions required to maintain the anthocyanin stability over a long period of time . investigating the effects of storage temperature on anthocyanin degradation will be highly beneficial because one of the vital steps in the procedure of manufacturing dsscs involves storage of the extracted pigments . in this study , special emphasis was paid to study the stability of promising pigments stored under different storage temperature regimes . brightly red / purple colored plant parts ( flowers , fruits , tubers , and leaves ) were harvested to determine the presence of anthocyanin ( table 1 ) . the anthocyanin extractions of the above plant parts were made following the procedure described by rodriguez - soana and wrolstad . 5  g of each freshly collected plant samples was used to extract the anthocyanin pigments . the pigments were initially extracted using 150  ml of 70% ethanol ( w / v% ) and stored overnight at 4c . on the following day , the extraction was mixed thoroughly by using a magnetic stirrer for two hours under air - conditioned room temperature ( 25c ) . the extraction was filtered using whatman 's ashless 110  mm filter paper to remove any solid residues . subsequently , the extracts were centrifuged at 4500  rpm using a denley bs400 ( uk ) centrifuge machine for five minutes to separate all residues . lastly the supernatant of the ethanolic extracts was gently mixed with equal volumes of petroleum ether to separate polar and nonpolar pigments . this component was carefully poured to a 10  ml glass bottle , tightly stoppered and wrapped in aluminum foil to avoid exposure to light and treatments for different temperature regimes . screening of separated anthocyanin pigments was done by measuring their absorbance spectra using uv - vis spectrophotometer ( shimadzu uv-1800 , japan ) . before the commencement of absorbance measurements , this acidification process converts anthocyanin derivatives to anthocyanidin that gives absorption spectra in the region of 490550  nm [ 11 , 15 , 16 ] . plant extracts that showed higher absorption spectra were selected for further investigations to evaluate the impacts of varying temperature regimes . all measurements were done in three replicates per sample . to finalize the sample selection for dsscs , those extracts that showed the highest uv - vis absorbance reading were chosen , and their anthocyanin contents were determined following the ph differential method described by giusti and wrolstad . anthocyanin content was calculated according to the following equation : 
 ( 1 )  anthocyanin  pigment  content = amwdf103l , 
 where a = ( a520nm  a700 nm ) ph 1.0  ( a520  nm  a700  nm ) ph 4.5 , mw  ( molecular  weight ) = 449.2  g / mol for cyanidin-3-glucoside , df = dilution factor ,  = 26900  l  mol  cm , 10 is the factor for converting g to mg , and l is the assumed path length in cm . aliquots of plant extracts were brought to ph 1 and 4.5 and allowed to equilibrate for one hour . the absorbance of each equilibrated solution was then measured at 520  nm ( max ) and 700  nm for haze correction . the mw used in this formula corresponds to the predominant anthocyanin in the sample . in some cases , predominant anthocyanin in a material however , throughout the years , there has been a lack of uniformity in the values of absorptivity of purified anthocyanin , mainly due to difficulties of obtaining pure crystalline anthocyanin in adequate quantities [ 11 , 17 ] . since there is a huge variety of anthocyanin spread in nature , it has been suggested that if the major anthocyanin is unknown , it can be expressed as cyanidin-3-glucoside because that is the most abundant anthocyanin in nature [ 11 , 12 , 1720 ] . the anthocyanin extracts of m. malabathricum , h. rosa - sinensis , and c. variegatum were stored in a tightly stoppered glass bottle fully covered with aluminum foil to avoid exposure to light . extracts were stored at three different storage temperatures , namely , 4c , 20c , and 25c , to evaluate the stability during storage . in order to determine the anthocyanin contents , the spectroscopic absorbance of the extracts were initially determined for three consecutive days followed by weekly measurements over a period of four months from september 2012 to january 2013 . the first - order reaction constant rate ( k ) and half - life ( t1/2 ) were calculated using the following equation : 
 ( 2)ln(ctco)=kt , t1/2=ln(0.5)k1 , 
 where co is the initial monomeric anthocyanin content and ct is the monomeric anthocyanin content after t minute storage at a given temperature . the anodes were dipped in the dye extract for overnight at room temperature ( 25c ) and dried out . the cell was assembled using dyesol 's test cell assembly machine with the surlyn ( 50  m , dyesol ) . the electrolyte solution containing tetrabutylammonium iodide ( tbai ; 0.5  m)/i2 ( 0.05  m ) , acetonitrile , and ethylene carbonate ( 6  :  4 , v / v )   was introduced through a predrilled hole in platinum counter electrode . the cell was kept under irradiation of about 3 - 4  h for light soaking . finally i - v characteristic of the dssc was measured under 1 sun level ( dyesol solar simulator lp-156b ) . the performance of dssc sensitized with anthocyanin pigments extracted from m. malabathricum , h. rosa - sinensis , and c. variegatum was evaluated by short circuit current ( jsc ) , open circuit voltage ( voc ) , fill factor ( ff ) , and energy conversion efficiency (  ) . the absorbance spectra of the dye adsorbed on tio2 electrodes were also measured . before the commencement of absorbance measurements , each of the tio2 electrodes were dipped in the dye extract overnight at room temperature ( 25c ) and air dried . as shown in figure 1 , the maximum absorbance of anthocyanin varied significantly in different species . jacaranda obtusifolia , licuala orbicularis , spinacia oleracea , and durantaerecta flower extracts showed no absorbance at 520  nm ; hence it can be concluded that they do not possess anthocyanin . among the rest , 17 other plant extracts showed maximum absorbance of 0.1 or lower and therefore they were not selected to further investigations . on the other hand , the remaining sample extracts showed absorbance maxima greater than 0.1 . however , only three species , each representing fruit , flower , and leaves ( melastoma malabathricum , hibiscus rosa - sinensis , and codiaeum variegatum ) , which showed that highest absorbance maxima were selected for further investigations . table 2 showed that among the samples investigated after preliminary screening , the highest anthocyanin concentration was found to be in the fruit pulp of m. malabathricum ( 8.43  mg l ) , followed by h. rosa - sinensis ( 4.63  mg  l ) then c. variegatum ( 2.22  mg all three extracts showed prominent peaks at 490550  nm after the extracts were acidified with hcl ( figure 2(a ) ) . this result indicated and proved once again that more anthocyanidin presents in the extracts [ 11 , 15 , 16 ] . on the other hand , figure 2(b ) showed that m. malabathricum extract exhibited the best absorbance after being adsorbed into the tio2 electrode . this extract also gave the best efficiencies in dsscs , while c. variegatum in tio2 gave the second best absorbance , followed by h. rosa - sinensis . the absorbance results of the dye adsorbed tio2 electrodes were consistent with i - v characteristics data . the storage temperature had a strong influence on the degradation of anthocyanins extracted from all three extracts ( see figure 3 and table 3 ) . the most distinctive pattern that was found in all three species was that anthocyanin pigments decreased progressively when stored at 25c over a three - month period . however the stability of all three pigments was relatively high when the temperature was maintained at 4c . the degradation rates are represented by the half - life values ; the higher the number , the more stable the anthocyanin extract . result showed significantly greater stability of anthocyanin in all three species when they were stored at 4c , and storage at 25c resulted in much faster degradation . the highest half - life periods for anthocyanin in m. malabathricum , h. rosa - sinensis , and c. variegatum were 540.77 , 571.19 , and 352.86 days at 4c , respectively , and it decreased rapidly to 110.71 , 219.74 , and 254.25 days at 25c over a period of three months . similar results were reported by janna et al . , who also studied the stability of melastoma malabathricum and found that the suitable storage condition for anthocyanin pigment is acidic solution in dark and low temperature ( 4c ) . the result of this investigation was also consistent with other similar studies where they found that anthocyanin pigments degrade faster as the temperature increases to 25c and the stability is maintained at low temperatures ( i.e. , 4c ) [ 12 , 21 , 23 ] . a previous study on the anthocyanin degradation in black carrot showed that the t1/2 value in shalgam drinks maintained at 4 and 25c were 34 and 11 weeks , respectively . a similar study also found that the t1/2 value of monomeric anthocyanin of black carrot showed a distinct difference of 71.8 and 18.7 weeks , respectively , when maintained at 4 and 20c , respectively . our investigation showed that frozen anthocyanin extracts maintained at 20c also ensure a good stability over a period of three months ; however , the best storage temperature was still 4c . the current - voltage characteristics of the dsscs sensitized with the anthocyanin pigment extracted from m. malabathricum fruit pulp , h. rosa - sinensis flowers , and c. variegatum leaves are shown in figure 4 . the conversion efficiencies (  ) of dsscs were 1.16 , 0.16 , and 1.08% , respectively ( table 4 ) . the highest effciency was obtained from dssc sensitized with m. malabathricum fruit pulp extract with the open curcuit voltage ( voc = 0.383  v ) , short curcuit current density ( isc = 6.17  ma / cm ) , and fill factor ( ff = 0.44 ) . natural pigments extracted from fruits and vegetables such as chlorophyll and anthocyanins have been extensively investigated as sensitizers for dsscs . by far , the best performance reported was obtained from beet roots with an efficiency of 2.71% [ 25 , 26 ] . other studies include punicagranatum , hibiscus sabdariffa , pomegranate juice , wild silicon prickly pear ( opuntia vulgaris ) , rhoeospathacea , mangosteen pericarp , red turnip , ficus reusa , and hibiscus surattensis with conversion efficiencies of 1.86 , 1.6 , 1.5 , 2.06 , 1.49 , 1.17 , 1.70 , 1.18 , and 1.14% , respectively [ 6 , 7 , 2731 ] . our study has shown that extract from m. malabathricum yielded the highest efficiency , 1.16% . the result is encouraging and the methods employed to maintain its stability is extremely promising . high efficiency obtained in the fruit pulps of m. malabathricum can be attributed to the carbonyl and hydroxyl groups of anthocyanin molecules present [ 3 , 6 , 7 , 25 ] . this ability favours photoelectric conversion as it allows effective binding with the surface of tio2 porous film . further improvements in refinement of extraction and application methods will no doubt increase the efficiency of this dye in dsscs . out of the 35 different species that were tested for the presence of anthocyanin pigments , melastoma malabathricum , hibiscus rosa - sinensis , and codiaeum variegatum were selected as potential candidates in dsscs . among the three species , m. malabathricum extract exhibited the highest anthocyanin content . based on the studies of anthocyanin stability on storage temperature , the three different species investigated , dye obtained from m. malabathricum fruit pulp also gave the highest efficiency . the photovoltaic performance of this dye was encouraging ( 1.16% ) . with further refinement of extraction and application methods , furthermore , due to the simple and cost - effective preparation techniques involved in the dye extraction of this species , it makes a promising alternative sensitizer for dsscs .
natural dyes have become a viable alternative to expensive organic sensitizers because of their low cost of production , abundance in supply , and eco - friendliness . 
 we evaluated 35 native plants containing anthocyanin pigments as potential sensitizers for dsscs . 
 melastoma malabathricum ( fruit pulp ) , hibiscus rosa - sinensis ( flower ) , and codiaeum variegatum ( leaves ) showed the highest absorption peaks . 
 hence , these were used to determine anthocyanin content and stability based on the impacts of storage temperature . 
 melastoma malabathricum fruit pulp exhibited the highest anthocyanin content ( 8.43  mg / l ) followed by h. rosa - sinensis and c. variegatum . 
 significantly greater stability of extracted anthocyanin pigment was shown when all three were stored at 4c . 
 the highest half - life periods for anthocyanin in m. malabathricum , h. rosa - sinensis , and c. variegatum were 541 , 571 , and 353 days at 4c . 
 these were rapidly decreased to 111 , 220 , and 254 days when stored at 25c . the photovoltaic efficiency of m. malabathricum was1.16% , while the values for h. rosa - sinensis and c. variegatum were 0.16% and 1.08% , respectively . 
 hence , m. malabathricum fruit pulp extracts can be further evaluated as an alternative natural sensitizer for dsscs .